research article investigating the degradability of hdpe ... e photodegradation of pe, such as the...
Post on 12-May-2020
Embed Size (px)
Research Article Investigating the Degradability of HDPE, LDPE, PE-BIO, and PE-OXO Films under UV-B Radiation
A. Martínez-Romo, R. González-Mota, J. J. Soto-Bernal, and I. Rosales-Candelas
Instituto Tecnológico de Aguascalientes, Avenida Adolfo López Mateos No. 1801 Ote, Fraccionamiento Bona Gens, 20256 Aguascalientes, AGS, Mexico
Correspondence should be addressed to R. González-Mota; firstname.lastname@example.org and J. J. Soto-Bernal; email@example.com
Received 12 August 2015; Revised 30 September 2015; Accepted 1 October 2015
Academic Editor: Javier Garcia-Guinea
Copyright © 2015 A. Mart́ınez-Romo et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The changes in structural properties of high density polyethylene films (HDPE), low density polyethylene films (LDPE), biodegradable polyethylene (PE-BIO), and oxodegradable polyethylene (PE-OXO) films exposed to UV-B radiation were studied. The carbonyl (𝐼CO) and vinyl (𝐼V) index, the crystalline phase fraction, and the dichroic ratio were used to evaluate the photooxidation of these polymers. The results obtained show that LDPE and HDPE undergo a major degree of oxidation and an increase in the crystalline phase fraction comparing to PE-BIO and PE-OXO. If the LDPE and HDPE are pretreated by an accurate radiation UV-B dosage before its different commercial uses or in its final disposition, they can become an option for biodegradable material without the necessity of adding organic agents or photosensitizers.
The widespread use of polyethylene PE as packaging films is due to its mechanical properties, enabling the production of mechanically strong films . These plastic films accumulate in the environment due to their low degradability, generating pollution and accumulating in landfills. Moreover, because the films have very small masses and are usually contami- nated, recycling is economically unfeasible .
Polyethylene has a simple and semicrystalline molecular structure, high molecular weight but does not easily degrade in the natural environment because it does not absorb UV radiation [3, 4]; however, the presence of impurities like catalyst remnants, plasticizers, and antioxidants can induce the PE to absorb UV-B radiation [5–8]. These properties that make plastics the material of choice for many applica- tions, particularly for single use packaging, together with an increase in usage have also created disposal problems at the end of the useful life of these products .
In recent years, due to the low rate of degradability of PE, the need for degradable PE has become a major topic of research, and hence organic molecules and prooxidants agents have been included in the molecular structure of
polyethylene, in order to obtain biodegradable (PE-BIO) and oxodegradable (PE-OXO) materials, respectively [9–12].
Degradation of polymers ismainly due to photooxidation and thermooxidation reactions [6, 7, 13, 14], causing the chain scission and cross-linking of polymer backbone, the formation of carbonyls (C=O) and vinyl (CH
2 =CH) groups,
and, finally, changes in the conformation and crystallinity of the polymer [15–17]. PE is a low degradability polymer because it is mainly composed of C–C and C–H bonds (𝜎 bonds) whose bond energy is in the order of 300–600 kJ/mol.
The principle of degradation states that the amount of energy absorbed by a molecule must exceed the bond energy in order to cause degradation. So, UV-A radiation energy is not enough to break the chemical bonds of the PE and cause the degradation of the polymer . UV-B radiation is particularly efficient in bringing about photodamage in synthetic polymers.
Although the UV-C has sufficient energy to break 𝜎 bonds, it is not a commonly used technique in the degrada- tion of plastics because plastics materials lost their mechan- ical properties; furthermore, the UV-C radiation emitted by the sun is absorbed by the atmosphere and does not reach the earth’s surface .
Hindawi Publishing Corporation Journal of Spectroscopy Volume 2015, Article ID 586514, 6 pages http://dx.doi.org/10.1155/2015/586514
2 Journal of Spectroscopy
IR spectroscopy is a useful technique for determining changes in the crystallinity degree of various polymers . The IR spectrum of semicrystalline PE presents a bifurcated band at 710–750 cm−1, rocking vibration of the methylene group (CH
2 ) from the amorphous and crystalline phase, as
well as a bifurcated band at 1450–1480 cm−1 which is due to the wagging vibration of the methylene (CH
2 ) group of the
crystalline phase [20, 21]. The orientation and conformation of the molecular
chains influence the mechanical properties of the polymers. The specificity of infrared absorption bands to particular chemical functional groups makes infrared spectroscopy especially attractive for measurement of chain orientation. For a given absorption band, the dichroic ratio is the param- eter commonly used to characterize the degree of optical anisotropy in stretched polymers. Dichroic ratio measure- ments require two different absorbance spectra of the sample, parallel (𝐴
‖ ) and perpendicular (𝐴
⊥ ) to the polymer stretch-
ing direction. The dichroic ratio is defined by 𝑅 = 𝐴 ‖ /𝐴 ⊥
[21–23]. The photodegradation of PE, such as the formation of
oxidation products, the loss of molecular weight, and the crystallinity, has been characterized by other authors using technics such as differential scanning calorimeter (DSC), electronic microscopy (SEM), X-ray diffraction (XRD), and infrared spectroscopy (FTIR) [5, 24–27]. In this paper, the effect of UV-B radiation in unmodified, LDPE and HDPE, and modified, PE-BIO and PE-OXO, PE films was evaluated by changes in carbonyl index, vinyl index, the crystalline phase fraction, and dichroic ratio.
2.1. Material. LDPE, HDPE, PE-BIO, and PE-OXO bags samples were obtained in supermarkets fromAguascalientes, Mexico. These bags were made in Mexico and are commer- cialized in LatinAmerica .These bagswere obtained from different suppliers in order to gather the most representative ones on the market.
128 samples, 40 × 50mm with a thickness of 0.05mm, of low density polyethylene (LDPE), high density polyethy- lene (HDPE), biodegradable polyethylene (PE-BIO), and oxodegradable polyethylene (PE-OXO), were analyzed.
2.2. Photodegradation of PE. PE films were irradiated with 3.5 × 10−4W/cm2 UV-B lamps (280 and 320 nm). Samples were mounted on racks at 5 cm from the lamp. Samples were analyzed by various techniques at regular time intervals (0, 5, 15, 30, 45, and 60 days).
2.3. Evaluation of Photodegradation. The photodegradation of the PE was characterized by IR spectroscopy with Atten- uated Total Reflectance (ATR), using a spectrophotometer Thermo Nicolet model iS10 with a Germanium mirror (Ge), and a resolution of 2 cm−1 in the range of 650–4000 cm−1.
2.3.1. Carbonyl Index. Carbonyl index (𝐼CO) was calculated using (1), the IR absorption band at 1740 cm−1 (𝐴
and stretching vibration of the carbonyl group (C=O); the absorbance at 1835 cm−1 (𝐴
(1835) ) is used as reference :
𝐼CO = (𝐴 (1740) − 𝐴 (1835) )
(0.008 ∗ 𝑡) , (1)
where 𝑡 is the thickness of the sample (mm).
2.3.2. Vinyl Index. Vinyl index (𝐼V) was calculated using (2), ratio of absorbance of the band on 909 cm−1 (𝐴
stretching vibration of the vinyl group (CH 2 =CH)
𝑛 , and
absorbance at 2020 cm−1 :
𝐼V = (𝐴 (909) )
(𝐴 (2020) ) . (2)
2.3.3. Crystalline Phase Fraction. The PE crystalline phase fraction (𝛼) was calculated from the integrated intensities of IR absorption bands of the methylene (CH
2 ) at 717 cm−1
(𝐼int(717)), amorphous phase fraction, and crystalline phase fraction, 730 cm−1 (𝐼int(730)), according to (3); the integrated intensities of the IR bands were calculated using a Gaussian fitting of these bands [19, 29]:
𝛼phase(𝑖) = Integrated areaphase(𝑖) Integrated areaall phases
2.3.4. Dichroic Ratio. The dichroic ratio of the PE exposed to UV-B radiation was calculated by using the IR absorbance at 1460 cm−1 corresponding to the wagging vibration of the methylene group (CH
2 ) of the PE crystalline phase .
3. Results and Discussion
3.1. Infrared Spectroscopy. The infrared spectra of LDPE, HDPE, PE-BIO, and PE-OXO without exposure to UV- B radiation are shown in Figure 1; these spectra show the IR bands characteristics of PE: the stretching vibration of Carbon-Hydrogen (CH) group of the main chain at 2772–3038 cm−1 and the wagging and rocking vibration of methylene (CH
2 ) at 1440–1490 cm−1 and 700–750 cm−1,
respectively [20, 30]. IR spectra of HDPE and PE-BIO show a single peak at 700–750 cm−1 and at 1440–1490 cm−1 because they are polymers of linear structure, while for LDPE and PE-OXO, these same bands are bifurcated because they are branched polymers.
The IR spectra of the PE-BIO films show an IR absorption at 1740 cm−1, stretching vibration of the carbonyl group (C=O), whereas the IR spectrum of the PE-OXO films shows an IR absorption band at 909 cm−1, stretching vibration of the vinyl group (CH
2 =CH); these functional groups are
chromophores groups and are consid